School of Electrical Engineering and Graduate School of Energy, Environment, Water, and Sustainability, Korea Advanced Institute of Science and Technology, 291 Daehak-ro, Yuseong-gu, Daejeon 305-701, Korea.
Based on first-principles approaches, we study the ballistic phonon transport properties of finite monatomic carbon chains stretched between graphene nanoribbons, an sp-sp2 hybrid carbon nanostructure that has recently seen significant experimental advances in its synthesis. We find that the lattice thermal conductance anomalously increases with tensile strain for the even-numbered carbon chains that adopt the alternating bond-length polyyne configuration. On the other hand, in the odd-numbered carbon chain cases, which assume the equal bond-length cumulene configuration, phonon conductance decreases with increasing strain. We show that the strong odd-even phonon transport effects originate from the characteristic longitudinal acoustic phonon modes of carbon wires and their unique strain-induced redshifts with respect to graphene nanoribbon phonon modes. The novel phonon transport properties and their atomistic mechanisms revealed in this work will provide valuable guidelines in de- signing hybrid carbon nanostructures for next-generation electronic, bio, and energy device applications.
1 fields significantly overestimate phonon transmissions across 1. Introduction GNR-atomic carbon contacts. In studying the ballistic phonon transport properties 1 Representing the ideal one-dimensional (1D) sp - of various GNR-CC-GNR junction models, we particularly hybridized carbon systems, monoatomic carbon chains (CCs) focus on the effects of tensile strain as well as the number of were predicted to exhibit intriguing physical and chemical carbon atoms within CCs. Strain was predicted to be an properties but their experimental investigations have been important variable that affects the structural and electronic 2 3 relatively slow compared to other sp - and sp -carbon properties of infinite[29-32] as well as finite CCs.[18, 33, 34] allotropes.[1-4] While the infinite CC or carbyne is not yet Regarding the number of C atoms within finite CCs, while observed and its existence still remains controversial, much strong odd-even effects were predicted for the structural and progress has been recently made in the experimental electron transport properties of GNR-CC-GNR junctions,[19 , realization of finite CC systems. An interesting aspect of this 22, 33, 34] it remains to be seen whether an oscillatory development is that, rather than the direct synthesis of behavior also appears in phonon transport and if does what its isolated molecular CCs,[5, 6] they were successfully prepared nature is. We will show that a strong strain-dependent odd- 1 2 in the sp -sp hybrid carbon structures. A notable case is the even phonon transport effect indeed arises because phonon CC confined within carbon nanotubes,[7, 8] and the other is conductances in the even-numbered (odd-numbered) CC the CC stretched between graphene.[9-17] junctions increase (decrease) with tensile strain. The effect is In particular, the graphene-CC-graphene system found in both armchair and zigzag GNRs, indicating the robust assumes an ideal electrode-channel-electrode junction nature of the effect. The microscopic mechanisms rationalized configuration,[9-17] providing unique opportunities to study by the polyynic atomic structure of even-numbered CCs and the quantum transport properties of all-carbon nanodevices. the strong redshifting behavior of their longitudinal optical (LO) The infinite CCs can adopt cumulene (∙∙∙ C=C=C=C ∙∙∙) or modes with respect to GNR phonon bands will become useful guidelines in designing hybrid carbon nanostructures for polyyne (∙∙∙ C≡C–C≡C ∙∙∙) configuration (Fig. 1a) and exhibit advanced device applications. metallic or semiconducting properties, respectively.[3, 4] In a notable example, very recently, strain-induced metal-to- insulator (i.e. cumulene-to-polyyne) transition was 2. Computational method observed, confirming another recent theoretical prediction. Another promising example theoretically suggested is spintronic applications such as spin filter and spin 2.1 Density-functional theory phonon calculations valve, which will be operated based on the spin-polarized nature of graphene zigzag edge states and can be modulated by Following our earlier works on stretched molecular the number of carbon atoms within CCs (cumulene or junctions,[35, 36] we carried out strain-dependent geometry polyyne).[19-21] optimizations within the local density approximation (LDA) of In this work, applying an atomistic Green’s function DFT implemented in the SIESTA package. Dynamical method (AGF) based on density functional theory (DFT) matrices were obtained with the DFT forces and the small calculations, we investigate the strain-dependent ballistic displacement method using the Phonopy code. Norm- phonon transport properties of CCs bridging graphene conserving pseudopotentials and double-zeta-plus-polarization nanoribbon (GNR) electrodes (Fig. 1b). Although several quality atomic orbital basis sets were adopted. The theoretical reports on the charge and spin transport properties convergence criterion for atomic forces was set to 10−3 eV/Å. of GNR-CC-GNR junctions have previously appeared,[19 , 22] study on their phonon transport properties is non-existent. 2.2 Quantum phonon transport calculations More generally, while ballistic electron and spin transports in nanoscale junctions have been extensively studied in the past decade or so, still much less is known about their ballistic For the computation of ballistic phonon transport phononic heat transport.[24, 25] We here adopt the properties, we used an in-house code that implements the microscopic AGF theory to describe the thermal resistance atomistic matrix Green’s function (MGF) formalism[23, 26-28] across the dimensionally mismatched sp1-sp2 interfaces.[26-28] and was developed based on our electronic MGF code.[35, 39, Moreover, in spite of the high computational cost, we will 40] We are concerned with the linear response limit, or when utilize first-principles atomics forces obtained through DFT the difference of the electrode 1/2 temperature 푇 / is very because it was shown in a previous study that classical force small, 푇 − 푇 ≪ 푇 ≡ (푇 + 푇 )/2. Then, after computing the phonon transmission function,
2 푇 (휔)=Tr[Γ (휔)G(휔)Γ (휔)G (휔)], (1) conclusions based on LDA or generalized gradient approximation will not be modified by employing hybrid functionals.[18, 30] Considering the increasing Peierls where G is the retarded Green`s function matrix of the channel distortion and strain effects within hybrid functionals, we region and Γ / is the broadening matrix resulting from the expect that the strain-dependent odd-even effects for the GNR- coupling of the channel with the electrode 1/2, we calculated CC-GNR junctions reported below will become more the lattice thermal conductance according to prominent in experimental situations. In Fig. 2, we summarize the characteristics of strain- ∞ 퐾 (푇) = ∫ ℏ휔푇(휔) , (2) dependent phonon properties of infinite CCs as well as 4zGNR. Analyzing the spatial decay of dynamical matrix elements (Fig. 2a upper panels), the force interaction range in CCs is found to where 푛 = [exp(ℏ휔/푘 푇)−1] is the Bose-Einstein be much longer than that in 4zGNRs. Particularly, we observe distribution function. that the interaction is extremely long-ranged for the cumulene chain, obtaining over the 10-2 eVÅ-2amu-1 level values for the 3. Results and Discussion off-diagonal dynamical matrix elements even at the 150 Å distance compared with the drop to the 10-4 eVÅ-2amu-1 level at about 70 Å (15 Å) for the polyyne (4zGNR) counterpart. 3.1 Phononic heat transport in infinite CCs. These characteristics show up in the phonon band structures of We first discuss the strain-dependent variations in the the cumulene chain as a Kohn anomaly (over bending of the lattice thermal transport properties of infinite CCs (carbyne) longitudinal acoustic (LA) phonon dispersion and the phonon and GNRs, which become the basis of analyzing the phonon softening) at the point of the polyyne Brillouin zone (or the transport in GNR-CC-GNR junctions. In terms of the atomic zone boundary at the cumulene Brillouin zone, Fig. 2b). On the structures of infinite carbynes, we obtained within LDA 1.269 other hand, in the polyyne case, the Peierls distortion opens a gap between the LA and LO branches at the zone boundary X Å (1.301 Å) as the C≡C (C–C) bond length in the polyyne form point. (Fig. 2a). The frequency ranges of infinite polyyne and 1.285 Å as the C=C bond length in the cumulene and cumulene phonon modes are extended up to about 2250 counterpart (Fig. 1a). Due to Peierls distortion that drives the cm-1 (Fig. 2a middle panels, dotted lines) and 2240 cm-1 (Fig. bond-length alternation and associated opening of a 2b middle panels, dotted lines), respectively, within our bandgap,[29, 30, 32] the polyyne structure should be calculations, and these high-frequency phonon modes are the energetically more stable than the cumulene counterpart and sources of experimentally observed Raman signals in the 1800 within our calculations the energy difference between the two – 2300 cm-1 spectral region.[42, 43] Note that no other carbon was of 1.12 meV per carbon atom. As the GNR electrodes, we nanostructure have Raman peaks in this region, so they become adopted the hydrogen-passivated four zigzag-chain zigzag the characteristic feature of sp-hybridized carbons. In terms GNR (4zGNR) and seven dimer-line armchair GNR (7aGNR) of thermal transmissions and conductance, we find that the with the optimized unit cell lattice constants of 2.460 Å and Kohn anomaly-related features result in 푇 (휔) of cumulene 4.260 Å, respectively (Fig. 1b). larger than that of polyyne over some frequency ranges Upon applying tensile strains, we find for the polyene (particularly up to ~ 1200 cm-1; Figs. 2a and 2b middle right case that the long C–C bond length increases faster than the panels, dotted lines) and thus the 퐾 (푇) values of cumulene short C–C bond length, or the preference for the polyyne enhanced over those of polyyne (Fig. 2a and 2b lower panels, configuration is enhanced with strain (Fig.1c).[30, 32] dotted lines). Quantifying the degree of polyynicity using the bond-length Next, applying tensile strains on the polyyne chain, alternation (BLA) value, defined as the difference between we find that the short triple bond length relatively remains short C≡C and long C–C bond lengths, we find that BLA constant while the long single bond length linearly increases increases from of 0.032 Å to 0.130 Å and to 0.207 Å as the (Fig. 1c). The large strain-induced decrease in force constants tensile strain increases from 0 % to 8 % and to 12 % (Fig. 1d). of alternating single bonds results in significant redshifts of LA The Peierls instability manifested in BLA is underestimated and LO modes and corresponding reduction of high-frequency within LDA, which incorrectly overestimates the tendency of range 푇 (휔) (Fig. 2a middle panels, dot-dahsed and solid electron delocalization due to its self-interaction error, and the lines), resulting in the decrease of 퐾 (푇) by ~ 38 % with 12 % deficiency could be corrected by employing more elaborate strain at 300 K (Fig. 2a lower panels, dot-dahsed and solid hybrid DFT functionals. However, such calculations are lines). For the cumulene case, we again observe a large-scale prohibitive for the large GNR-CC-GNR junction models, and redshift of 푇 (휔) corresponding to the LA mode in the high- more importantly one can expect that the qualitative
3 frequency region, and it in turn results in a ~ 27 % reduction of To explain the microscopic mechanisms of the strain-
퐾 (푇) with 12 % strain at 300 K (Fig. 2b, dot-dahsed and induced increase (decrease) in 퐾 (푇) for even-numbered solid lines). (odd-numbered) CC junctions, we analyzed the atomic structures, phonon transmissions, and projected density of For the cases of 4zGNR (Fig. 2c) and 7aGNR (Fig. states (PDOS) at the unstrained and strained conditions shown S1), the frequency ranges of their phonons reaching up to ~ in Fig. 4. Note that as shown in Fig. 5 we obtain essentially 1680 cm-1 and ~ 1690 cm-1, respectively, are lower than those identical results for the 7aGNR case. To begin with, observing of CCs extending up to ~ 2250 cm-1. Moreover, due to the the optimized atomic structures of GNR-CC-GNR junctions in structural rigidity of the hexagonal arrangement of sp2 carbon detail (see Figs. S3 and S4), we find that the even-numbered atoms, the degree of strain-induced phonon band flattening or (odd-numbered) CCs stretched between GNRs adopt the redshift of high-frequency 푇 (휔) is smaller for GNRs, alternated polyyne-like (equalized cumulene-like) structures. amounting to the 퐾 (푇) reductions of ~ 14% and ~ 11% in the In addition, compared with the infinite carbyne limits, we 4zGNR and 7aGNR, respectively. observe that the finite CCs in junction models are in effectively strained conditions (Figs. 1c and 1d). Moreover, due to the 3.2 Phononic heat transport in infinite CCs. differences in their structural rigidity, we find that the effective strain induced onto the GNR regions is relatively negligible We now move on to consider the phonon transport compare to that of CCs. properties of CCs stretched between two GNR electrodes, which is the main focus of this work. Different from the infinite Moving on to the 푇 (휔) spectra of eight-carbon (8C) carbyne limit, the ideal case where Peierls distortion could be wire bridging 4zGNR electrodes, we immediately notice that -1 rigorously defined, the structural and electronic properties of 푇 (휔) values at cm are significantly enhanced finite CCs such as BLA, electronic band gap, and vibrational with strain (Fig. 4a, blue down arrows). On the other hand, properties are strongly affected by the length and termination -1 such 푇 (휔) enhancement at cm is absent for the of CCs.[3, 33] Inserting several odd- and even-numbered CCs 7C chain case (Fig. 4b), explaining the strong strain-induced between 4zGNR or 7aGNR electrodes, we first prepared a odd-even effects in 퐾 (푇) of GNR-CC-GNR junctions. The series of GNR-CC-GNR junction models (Fig. 1b). Each origins of different strain-induced 푇 (휔) changes in the junction model was once more optimized with DFT and then -1 its dynamical matrices were calculated to extract coherent cm frequency region can be understood by analyzing phonon transport properties. For the strained junction models, the phonon PDOS projected onto CCs. As emphasized earlier, the electrode-region GNRs were stretched by L = 0.8 Å and the high-frequency LO phonon modes of polyyne chains are once again the DFT-phonon MGF calculations were repeated. discriminated from those of other carbon-based More computational details can be found in the Computational nanostructures, and particularly they are strongly redshifted method section and Fig. S2. with increasing tensile strain (Fig. 2). Although the 8C chain within the unstrained junction is in an effectively strained state with reference to the infinite polyyne case (5.8 % in terms of The results summarized in Fig. 3 strikingly show that the bond lengths of central carbon atoms), the 8C chain LO we obtain the opposite strain-induced 퐾 (푇) variation trends mode is still located above the 4zGNR phonon states (Fig. 4a, for the even-numbered and odd-numbered CCs. The strong upper panels). However, upon applying additional strain to the odd-even effect becomes a robust feature at T > ~ 100 K and is 4zGNR-8C-4zGNR junction, the 8C chain LO mode is further observed for varying number of carbon atoms (N ) as well as C redshifted, making the spectral ranges of the 8C chain and for both 4zGNR and 7aGNR electrode cases, indicating its 4zGNR phonons overlap with each other and accordingly robustness and universality in the GNR-CC-GNR junction -1 increasing 푇 (휔) at cm significantly (Fig. 4a, configuration. The overall reduction of 퐾 (푇) in junction lower panels). models compared with that in infinite carbynes can be understood in view of the introduction of two GNR-CC sp2-sp1 The spatially well-delocalized nature is a necessary contacts. In addition, considering the reduction of 퐾 (푇) with condition for a transmission eigenmode to support efficient increasing tensile strain in carbynes and GNRs (Fig. 2), the quantum transport, and the visualization of eigenstates of the strain-induced 퐾 (푇) reduction in odd-numbered CC is molecular projected Hamiltonian has well established such a reasonable. On the other hand, the strain-induced enhancement criterion in the electron quantum transport case.[44, 45] In a of 퐾 (푇) in even-numbered CC cases cannot be understood similar spirit, we visualized the vibrational modes (phonon using the infinite carbyne data, implying it originates from the local PDOS) corresponding to the enhanced transmission peak unique interactions between finite-CC and GNR phonons. at 1490 cm-1 in the unstrained and strained 8C junction cases, and they indeed clearly show the absence and activation
4 of CC phonon modes in the former and latter cases, This work was supported by the Nano-Material Technology respectively (Fig. 4a, right panels). For the 7C chain case, on Development Program (Nos. 2016M3A7B4024133 and the other hand, such strain-induced transition behavior is less 2016M3A7B4909944), Basic Research Program (No. 2017R1A2B3009872), Global Frontier Program (No. noticeable (Fig. 4b, right panels). The 7C chain mode at 2013M3A6B1078881), and Basic Research Lab Program (No. -1 1490 cm is already activated within the unstrained 4zGNR- 2016M3A7B4909944) of the National Research Foundation 8C-4zGNR junction configuration, and correspondingly the funded by the Ministry of Science and ICT of Korea. transmission and CC PDOS peaks are present in Fig. 4b upper left panels. Such difference between even- and odd-number CC cases can be simplistically understood in terms of the slightly Corresponding Author Information more strained condition for the odd-numbered CCs with reference to the infinite cumulene limit (6.5 % in terms of the *Y.-H.K.: [email protected] bond lengths of central carbon atoms). However, more detailed analysis indicates that odd-numbered CC cases correspond to a complex situation where the mapping to cumulene is not Keywords strictly valid (e.g. the C-C bonds adjacent to GNRs are single- bonded rather than double-bonded; see Figs. S3 and S4), and phonon quantum transport, carbon atom chains, graphene we believe it deserves more close examinations in combination nanoribbon, first-principles simulation with the electronic structures of different sp-sp2 contacts in the future.[17, 33]
In summary, we carried out ab initio phonon transport calculations on finite monatomic CCs stretched between GNR electrodes. Representing the ultimate all-carbon junction model, these hybrid carbon nanostructures based on sp-sp2 interfaces are appealing in many aspects but the research efforts have been so far limited to their structural and electronic (and spin) transport properties. Systematically considering a series of CC channels and both zGNR and aGNR electrodes, we found that the phonon conductance of the sp-sp2 hybrid structures exhibits strong odd-even oscillations. Specifically, while odd-numbered CCs adopted the cumulenic structure and showed the phonon conductance decrease with increasing tensile strain, even-numbered CCs assumed the polyynic configuration and anomalously showed the strain-induced conductance increase. The strong odd-even ballistic phonon transport effects were rationalized in terms of the strain- dependent behavior of polyyne LO phonon modes, which are characteristic to sp-hybridized CCs and exhibit stronger redshifts than the high-frequency phonon modes of sp2 carbons in GNRs. Combined with the electron and spin transport properties that were also predicted to show oscillatory behaviors,[19 , 22] the strong odd-even phonon transport effects could open up novel opportunities in advanced nano- device applications.
5 References  J.A. Fürst, M. Brandbyge, A.P. Jauho, Atomic carbon chains as spin-transmitters: An ab initio transport study, Epl-Europhys.  R.B. Heimann, S.E. Evsvukov, Y. Koga, Carbon allotropes: Lett. 2010;91:37002. a suggested classification scheme based on valence orbital  M.G. Zeng, L. Shen, Y.Q. Cai, Z.D. Sha, Y.P. Feng, Perfect hybridization, Carbon 1997;35(10-11):1654-1658. spin-filter and spin-valve in carbon atomic chains, Appl. Phys. Lett.  A. Hirsch, The era of carbon allotropes, Nat. Mater. 2010;96:042104. 2010;9(11):868-71.  L. Shen, M. Zeng, S.W. Yang, C. Zhang, X. Wang, Y. Feng,  C.S. Casari, M. Tommasini, R.R. Tykwinski, A. Milani, Electron transport properties of atomic carbon nanowires between Carbon-atom wires: 1-D systems with tunable properties, Nanoscale graphene electrodes, J. Am. Chem. Soc. 2010;132:11481-6. 2016;8:414-35.  B.K. Nikolic, K.K. Saha, T. Markussen, K.S. Thygesen,  F. Banhart, Chains of carbon atoms: A vision or a new First-principles quantum transport modeling of thermoelectricity in nanomaterial?, Beilstein J. Nanotechnol. 2015;6:559-69. single-molecule nanojunctions with graphene nanoribbon electrodes,  W.A. Chalifoux, R.R. Tykwinski, Synthesis of polyynes to J. Comput. Electron. 2012;11:78-92. model the sp-carbon allotrope carbyne, Nat. Chem. 2010;2(11):967-  Y. Dubi, M. Di Ventra, Colloquium: Heat flow and 71. thermoelectricity in atomic and molecular junctions, Rev. Mod. Phys.  J.A. Januszewski, R.R. Tykwinski, Synthesis and properties 2011;83:131-155. of long [n]cumulenes (n >/= 5), Chem. Soc. Rev. 2014;43(9):3184-  N. Li, J. Ren, L. Wang, G. Zhang, P. Hänggi, B. Li, 203. Colloquium: Phononics: Manipulating heat flow with electronic  X. Zhao, Y. Ando, Y. Liu, M. Jinno, T. Suzuki, Carbon analogs and beyond, Rev. Mod. Phys. 2012;84:1045-1066. nanowire made of a long linear carbon chain inserted inside a  N. Mingo, L. Yang, Phonon transport in nanowires coated multiwalled carbon nanotube, Phys. Rev. Lett. 2003;90(18):187401. with an amorphous material: An atomistic Green’s function approach,  L. Shi, P. Rohringer, K. Suenaga, Y. Niimi, J. Kotakoski, Phys. Rev. B 2003;68:245406. J.C. Meyer et al., Confined linear carbon chains as a route to bulk  T. Yamamoto, K. Watanabe, Nonequilibrium Green's carbyne, Nat. Mater. 2016;15(6):634-9. function approach to phonon transport in defective carbon nanotubes,  B. Standley, W. Bao, H. Zhang, J. Bruck, C.N. Lau, M. Phys. Rev. Lett. 2006;96:255503. Bockrath, Graphene-based atomic-scale switches, Nano Lett.  J.-S. Wang, J. Wang, N. Zeng, Nonequilibrium Green’s 2008;8:3345-9. function approach to mesoscopic thermal transport, Phys. Rev. B  C. Jin, H. Lan, L. Peng, K. Suenaga, S. Iijima, Deriving 2006;74:033408. carbon atomic chains from graphene, Phys. Rev. Lett.  S. Tongay, R.T. Senger, S. Dag, S. Ciraci, Ab-initio electron 2009;102:205501. transport calculations of carbon based string structures, Phys. Rev.  A. Chuvilin, J.C. Meyer, G. Algara-Siller, U. Kaiser, From Lett. 2004;93:136404. graphene constrictions to single carbon chains, New J. Phys.  S. Cahangirov, M. Topsakal, S. Ciraci, Long-range 2009;11:083019. interactions in carbon atomic chains, Phys. Rev. B 2010;82:195444.  H. Zhang, W. Bao, Z. Zhao, J.W. Huang, B. Standley, G.  O. Cretu, A.R. Botello-Mendez, I. Janowska, C. Pham-Huu, Liu et al., Visualizing electrical breakdown and ON/OFF states in J.C. Charlier, F. Banhart, Electrical transport measured in atomic electrically switchable suspended graphene break junctions, Nano carbon chains, Nano Lett. 2013;13:3487-93. Lett. 2012;12:1772-5.  M. Liu, V.I. Artyukhov, H. Lee, F. Xu, B.I. Yakobson,  G. Casillas, A. Mayoral, M. Liu, A. Ponce, V.I. Artyukhov, Carbyne from first principles: chain of C atoms, a nanorod or a B.I. Yakobson et al., New insights into the properties and interactions nanorope, ACS Nano 2013;7:10075-82. of carbon chains as revealed by HRTEM and DFT analysis, Carbon  L. Ravagnan, N. Manini, E. Cinquanta, G. Onida, D. 2014;66:436-441. Sangalli, C. Motta et al., Effect of axial torsion on sp carbon atomic  A. La Torre, A. Botello-Mendez, W. Baaziz, J.C. Charlier, wires, Phys. Rev. Lett. 2009;102:245502. F. Banhart, Strain-induced metal-semiconductor transition observed  B. Akdim, R. Pachter, Switching behavior of carbon chains in atomic carbon chains, Nat. Commun. 2015;6:6636. bridging graphene nanoribbons: effects of uniaxial strain, ACS Nano  S.G. Sarwat, P. Gehring, G. Rodriguez Hernandez, J.H. 2011;5:1769-74. Warner, G.A.D. Briggs, J.A. Mol et al., Scaling Limits of Graphene  Y.-H. Kim, Toward Numerically Accurate First-Principles Nanoelectrodes, Nano Lett. 2017;17:3688-3693. Calculations of Nano-Device Charge Transport Characteristics: The  Y.C. Lin, S. Morishita, M. Koshino, C.H. Yeh, P.Y. Teng, Case of Alkane Single-Molecule Junctions, J. Kor. Phys. Soc. P.W. Chiu et al., Unexpected Huge Dimerization Ratio in One- 2008;52:1181-1186. Dimensional Carbon Atomic Chains, Nano Lett. 2017;17:494-500.  Y.-H. Kim, H.S. Kim, J. Lee, M. Tsutsui, T. Kawai,  F. Ben Romdhane, J.-J. Adjizian, J.-C. Charlier, F. Banhart, Stretching-Induced Conductance Variations as Fingerprints of Electrical transport through atomic carbon chains: The role of contacts, Contact Configurations in Single-Molecule Junctions, J. Am. Chem. Carbon 2017;122:92-97. Soc. 2017;139:8286-8294.  V.I. Artyukhov, M. Liu, B.I. Yakobson, Mechanically  J.M. Soler, E. Artacho, J.D. Gale, A. Garcia, J. Junquera, P. induced metal-insulator transition in carbyne, Nano Lett. Ordejon et al., The SIESTA method for ab initio order-N materials 2014;14:4224-9. simulation, J. Phys.: Condens. Matter 2002;14:2745-2779.  Z. Zanolli, G. Onida, J.C. Charlier, Quantum spin transport  A. Togo, L. Chaput, I. Tanaka, G. Hug, First-principles in carbon chains, ACS Nano 2010;4:5174-80. phonon calculations of thermal expansion inTi3SiC2,Ti3AlC2, and Ti3GeC2, Phys. Rev. B 2010;81:174301.
6  Y.-H. Kim, S.S. Jang, Y.H. Jang, W.A. Goddard III, First-  L. Ravagnan, P. Piseri, M. Bruzzi, S. Miglio, G. Bongiorno, principles study of the switching mechanism of catenane molecular A. Baserga et al., Influence of cumulenic chains on the vibrational and electronic devices, Phys. Rev. Lett. 2005;94:156801. electronic properties of sp-sp2 amorphous carbon, Phys. Rev. Lett.  Y.-H. Kim, J. Tahir-Kheli, P.A. Schultz, W.A. Goddard III, 2007;98:216103. First-principles approach to the charge-transport characteristics of  J. Heurich, J.C. Cuevas, W. Wenzel, G. Schon, Electrical monolayer molecular-electronics devices: Application to transport through single-molecule junctions: from molecular orbitals hexanedithiolate devices, Phys. Rev. B 2006;73:235419. to conduction channels, Phys. Rev. Lett. 2002;88(25 Pt 1):256803.  S.S. Kim, H.S. Kim, H.S. Kim, Y.-H. Kim, Conductance  G.I. Lee, J.K. Kang, Y.-H. Kim, Metal-Independent recovery and spin polarization in boron and nitrogen co-doped Coherent Electron Tunneling through Polymerized Fullerene Chains, graphene nanoribbons, Carbon 2015;81:339-346. J. Phys. Chem. C 2008;112:7029-7035.  L. Ravagnan, F. Siviero, C. Lenardi, P. Piseri, E. Barborini, P. Milani et al., Cluster-beam deposition and in situ characterization of carbyne-rich carbon films, Phys. Rev. Lett. 2002;89:285506.
Figure 1 | Atomic structures of DFT-optimized (a) polyyne (upper) and cumulene (lower), and (b) 4zGNR and 7aGNR. Schematics of GNR-CC junction contacts are shown together. Here, the red rectangles represent the primitive unit cells. (c) The bond lengths of the finite CC parts within the GNR-CC-GNR junction models are mapped to the bond lengths of infinite polyyne (solid lines) and cumulene (dotted line) at varying strain. Circles (squares) represent 4zGNR (7aGNR) cases. (d) The BLA values of even-numbered CC junctions mapped onto the infinite polyyne BLA values at varying strain. For the junction models, the bond length and BLA values are measured for the innermost carbon atoms.
Figure 2 | Density plots of the dynamical matrices (upper panels), strain-dependent phonon band structures (middle left panels), phonon transmissions (middle right panels), and thermal conductance (lower panels) of (a) polyyne, (b) cumulene, and (c) 4zGNR. For the density plots, left and right panels are from 0% and 8% strain conditions, respectively. Each axis represents the number of unit cells (UCs). The magnitude of matrix elements are given in the units of eVÅ-2amu-1. For the polyyne and cumulene cases, black dashed, green dash-dot, and red solid lines represent the 0, 8, and 12% strain conditions, respectively. For the zGNR case, black dashed and green solid lines represent the 0 and 8% strain conditions, respectively.
Figure 3 | Strain-dependent lattice thermal conductances of the representative GNR-CC-GNR junction models. Black dotted and blue solid lines represent the unstrained (dashed lines) and strained (solid lines) conditions, respectively. Effective strain values for the innermost carbon atoms in reference to infinite polyyne and cumulene structures are given for the even-numbered and odd-numbered CC cases, respectively. (b) Compilation of strain-dependent lattice thermal conductance with different number of carbon atoms for the 4zGNR (left) and 7aGNR (right) cases. Black dotted and solid lines represent the unstrained and strained conditions, respectively.
Figure 4 | Phonon transmissions (left upper panels), vibrational PDOS (left lower panels), and local phonon modes (right panels) at ≈1490 cm-1 in the (a) 4zGNR-8C-4zGNR and (b) 4zGNR-7C-4zGNR junction models for the unstrained (upper panels) and strained (lower panels) conditions. Effective strain values for the innermost CC atoms in reference to infinite polyyne and cumulene structures are given for the 8C and 7C cases, respectively. In the phonon PDOS red and grey lines represent the CC and GNR PDOS, respectively. In the transmission and PDOS data, blue down arrows indicate the frequency where local phonon mode is visualized (≈1490 cm-1). In the local phonon mode plots, black arrows represent the in-plane vibrational directions of each atom.
Figure 5 | Phonon transmissions, vibrational PDOS, and real-space visualizations of ≈1490 cm-1 phonon modes in the (a) 7aGNR-6C-7aGNR and (b) 7aGNR-5C-7aGNR junction models for the unstrained (upper panels) and strained (lower panels) conditions. Effective strain values for the innermost CC atoms in reference to infinite polyyne and cumulene structures are given for the 6C and 5C cases, respectively. Red and grey filled lines in the PDOS plots represent the PDOS of CC and GNR parts, respectively. Blue down arrows indicate the frequency near ≈1490 cm-1. In the local phonon mode plots, black arrows represent the in-plane vibrational directions of each atom.